LMucko/crystallography-open-database huggingface dataset:
Crystal structure and isothermal compression of Fe2O3, Cr2O3, and V2O3 to 50 kbars Note: P = 18.3 kbar
Finger, L. W.; Hazen, R. M.; Journal of Applied Physics 51 (1980) 5362–5367; doi:10.1063/1.327451

data_9016535
_publ_section_title
;
 Crystal structure and isothermal compression of Fe2O3, Cr2O3, and V2O3 to 50 kbars
 Note: P = 18.3 kbar
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              5362
_journal_page_last               5367
_journal_paper_doi               10.1063/1.327451
_journal_volume                  51
_journal_year                    1980
_chemical_compound_source        Synthetic
_chemical_formula_sum            'O3 V2'
_chemical_name_mineral           Karelianite
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   4.9322
_cell_length_b                   4.9322
_cell_length_c                   13.991
_cell_formula_units_Z            6
_cell_volume                     294.755
_database_code_amcsd             0017742
_exptl_crystal_density_diffrn    5.066
_cod_original_sg_symbol_H-M      'R -3 c'
_cod_original_formula_sum        'V2 O3'
_cod_database_code               9016535
Povondraite, a redefinition of the tourmaline ferridravite Note: Atomic parameters updated by Grice on 11/20/2001
Grice, J. D.; Ercit, T. S.; Hawthorne, F. C.; American Mineralogist 78 (1993) 433–436; doi:

data_9016536
_publ_section_title
;
 Povondraite, a redefinition of the tourmaline ferridravite
 Note: Atomic parameters updated by Grice on 11/20/2001
;
_journal_name_full               'American Mineralogist'
_journal_page_first              433
_journal_page_last               436
_journal_volume                  78
_journal_year                    1993
_chemical_compound_source        'San Francisco mine, Villa Tunari, Bolivia'
_chemical_formula_sum
'Al0.3 B3 Fe6.87 H3.12 K0.2 Mg1.83 Na0.8 O31 Si6'
_chemical_name_mineral           Povondraite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   16.186
_cell_length_b                   16.186
_cell_length_c                   7.444
_cell_volume                     1688.947
_database_code_amcsd             0001555
_exptl_crystal_density_diffrn    3.429
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'(Na.8 K.2) Fe6.87 Mg1.83 Al.3 Si6 B3 O31 H3.12'
_cod_database_code               9016536
The Structure and Formula of 12-Phosphotungstic Acid _cod_database_code 1010873
Keggin, J.; Proceedings of the Royal Society of London 144 (1934) 75–100; doi:

data_9016537
_publ_section_title
;
 The Structure and Formula of 12-Phosphotungstic Acid
 _cod_database_code 1010873
;
_journal_name_full               'Proceedings of the Royal Society of London'
_journal_page_first              75
_journal_page_last               100
_journal_volume                  144
_journal_year                    1934
_chemical_formula_sum            'O40 P W12'
_space_group_IT_number           224
_symmetry_space_group_name_Hall  'P 4n 2 3 -1n'
_symmetry_space_group_name_H-M   'P n -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   12.141
_cell_length_b                   12.141
_cell_length_c                   12.141
_cell_formula_units_Z            2
_cell_volume                     1789.631
_database_code_amcsd             0017544
_exptl_crystal_density_diffrn    5.339
_cod_duplicate_entry             1010873
_cod_original_cell_volume        1789.630
_cod_original_sg_symbol_H-M      'P n 3 m'
_cod_original_formula_sum        'P O40 W12'
_cod_database_code               9016537
_amcsd_formula_title             'H3 O40 P W12'
Les Perovskites (Ca1-x Srx) (Ca.3333 Nb.6667) O3 _cod_database_code 1001072
Hervieu, M.; Raveau, B.; Journal of Solid State Chemistry 28 (1979) 209–222; doi:10.1016/0022-4596(79)90073-2

data_9016538
_publ_section_title
;
 Les Perovskites (Ca1-x Srx) (Ca.3333 Nb.6667) O3
 _cod_database_code 1001072
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              209
_journal_page_last               222
_journal_paper_doi               10.1016/0022-4596(79)90073-2
_journal_volume                  28
_journal_year                    1979
_chemical_formula_sum            'Ca0.667 Nb1.333 O6 Sr2'
_space_group_IT_number           81
_symmetry_space_group_name_Hall  'P -4'
_symmetry_space_group_name_H-M   'P -4'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.19
_cell_length_b                   8.19
_cell_length_c                   8.209
_cell_formula_units_Z            4
_cell_volume                     550.628
_database_code_amcsd             0013365
_exptl_crystal_density_diffrn    5.088
_cod_duplicate_entry             1001072
_cod_original_formula_sum        'Sr2 Ca.667 Nb1.333 O6'
_cod_database_code               9016538
_amcsd_formula_title             'Ca0.3333 Nb0.6667 O3 Sr'
Stability, thermal behaviour, and crystal structure of ion ordered Bi1-xLnxO1.5 phases (Ln = Sm - Dy) _cod_database_code 1004122
Drache, M.; Conflant, P.; Obbade, S.; Wignacourt, J.; Watanabe, A.; Journal of Solid State Chemistry 129 (1997) 98–104; doi:10.1006/jssc.1996.7236

data_9016539
_publ_section_title
;
 Stability, thermal behaviour, and crystal structure of ion ordered
 Bi1-xLnxO1.5 phases (Ln = Sm - Dy)
 _cod_database_code 1004122
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              98
_journal_page_last               104
_journal_paper_doi               10.1006/jssc.1996.7236
_journal_volume                  129
_journal_year                    1997
_chemical_formula_sum            'Bi5.198 Gd2.802 O12'
_space_group_IT_number           199
_symmetry_space_group_name_Hall  'I 2b 2c 3'
_symmetry_space_group_name_H-M   'I 21 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   11.0488
_cell_length_b                   11.0488
_cell_length_c                   11.0488
_cell_formula_units_Z            4
_cell_volume                     1348.793
_database_code_amcsd             0013918
_exptl_crystal_density_diffrn    8.465
_cod_duplicate_entry             1004122
_cod_database_code               9016539
_amcsd_formula_title             'Bi0.65 Gd0.35 O1.5'
Laurentianite, [NbO(H2O)]3(Si2O7)2[Na(H2O)2]3, a new mineral from Mont Saint-Hilaire, Quebec: description, crystal-structure determination and paragenesis
Haring, M. M. M.; McDonald, A. M.; Cooper, M. A.; Poirier, G. A.; The Canadian Mineralogist 50 (2012) 1265–1280; doi:10.3749/canmin.50.5.1265

data_9016540
_publ_section_title
;
 Laurentianite, [NbO(H2O)]3(Si2O7)2[Na(H2O)2]3, a new mineral from Mont
 Saint-Hilaire, Quebec: description, crystal-structure determination and paragenesis
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1265
_journal_page_last               1280
_journal_paper_doi               10.3749/canmin.50.5.1265
_journal_volume                  50
_journal_year                    2012
_chemical_compound_source        'Mont Saint-Hilaire, Quebec, Canada'
_chemical_formula_sum            'H18 Na2.76 Nb3 O26 Si4'
_chemical_name_mineral           Laurentianite
_space_group_IT_number           143
_symmetry_space_group_name_Hall  'P 3'
_symmetry_space_group_name_H-M   'P 3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   9.937
_cell_length_b                   9.937
_cell_length_c                   7.004
_cell_volume                     598.946
_database_code_amcsd             0019711
_exptl_crystal_density_diffrn    2.464
_cod_original_formula_sum        'Na2.76 Nb3 Si4 O26 H18'
_cod_database_code               9016540
Die Kristallstrukturen einiger Hexachlorokomplexsalze. _cod_database_code 1010178
Engel, G.; Zeitschrift fur Kristallographie 90 (1935) 341–373; doi:

data_9016541
_publ_section_title
;
 Die Kristallstrukturen einiger Hexachlorokomplexsalze.
 _cod_database_code 1010178
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              341
_journal_page_last               373
_journal_volume                  90
_journal_year                    1935
_chemical_formula_sum            'Cl6 N2 Pb'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.135
_cell_length_b                   10.135
_cell_length_c                   10.135
_cell_formula_units_Z            4
_cell_volume                     1041.049
_database_code_amcsd             0017114
_exptl_crystal_density_diffrn    2.858
_cod_duplicate_entry             1010178
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        'Pb N2 Cl6'
_cod_database_code               9016541
_amcsd_formula_title             'Cl6 H8 N2 Pb'
Oscillatory zoned liddicoatite from Anjanabonoina, central Madigascar. I. Crystal chemistry and structure by SREF and 11B and 27Al MAS NMR spectroscopy Sample: L11, ordered model
Lussier, A. J.; Abdu, Y.; Hawthorne, F. C.; Michaelis, V. K.; Aguiar, P. M.; Kroeker, S.; The Canadian Mineralogist 49 (2011) 63–88; doi:10.3749/canmin.49.1.63

data_9016542
_publ_section_title
;
 Oscillatory zoned liddicoatite from Anjanabonoina, central Madigascar.
 I. Crystal chemistry and structure by SREF and 11B and 27Al MAS NMR spectroscopy
 Sample: L11, ordered model
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              63
_journal_page_last               88
_journal_paper_doi               10.3749/canmin.49.1.63
_journal_volume                  49
_journal_year                    2011
_chemical_compound_source        'Anjanabonoina, central Madagascar'
_chemical_formula_sum
'Al7.167 B3 Ca0.441 F0.681 Fe0.027 H3.319 Li1.278 Mn0.531 Na0.471 O30.319 Pb0.025 Si6'
_chemical_name_mineral           Fluor-liddicoatite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   15.8675
_cell_length_b                   15.8675
_cell_length_c                   7.1135
_cell_formula_units_Z            3
_cell_volume                     1551.069
_database_code_amcsd             0018418
_exptl_crystal_density_diffrn    3.112
_cod_original_cell_volume        1551.068
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'Ca.441 Na.471 Pb.025 Al7.167 Fe.027 Mn.531 Li1.278 Si6 B3 F.681 O30.319 H3.319'
_cod_database_code               9016542
Fluorbritholite-(Y), (Y,Ca,Ln)5[(Si,P)O4]3F, a new mineral of the britholite group
Pekov, I. V.; Zubkova, N. V.; Chukanov, N. V.; Husdal, T. A.; Zadov, A. E.; Pushcharovsky, D. Y.; Neues Jahrbuch fur Mineralogie, Abhandlungen 188 (2011) 191–197; doi:

data_9016543
_publ_section_title
;
 Fluorbritholite-(Y), (Y,Ca,Ln)5[(Si,P)O4]3F, a new mineral of the britholite group
;
_journal_name_full               'Neues Jahrbuch fur Mineralogie, Abhandlungen'
_journal_page_first              191
_journal_page_last               197
_journal_volume                  188
_journal_year                    2011
_chemical_compound_source        'Lagmannsvik, Hamaroy, Nordland, Norway'
_chemical_formula_sum
'Ca1.52 Ce0.35 Dy0.15 Er0.15 F Gd0.12 La0.06 Mn0.03 Nd0.33 O12 Pr0.06 Si3 Sm0.12 Y1.96 Yb0.18'
_chemical_name_mineral           Fluorbritholite-(Y)
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   9.4437
_cell_length_b                   9.4437
_cell_length_c                   6.8169
_cell_volume                     526.504
_database_code_amcsd             0018905
_exptl_crystal_density_diffrn    4.813
_cod_original_formula_sum
'Y1.96 Ca1.52 Ce.35 La.06 Nd.33 Yb.18 Dy.15 Er.15 Gd.12 Sm.12 Pr.06 Mn.03 Si3 O12 F'
_cod_database_code               9016543
Synthese et caracterisation de nouvelles phases du diagramme (K ou Na)-Bi-O _cod_database_code 1004129
Trehoux, J.; Abraham, F.; Thomas, D.; Materials Research Bulletin 17 (1982) 1235–1243; doi:10.1016/0025-5408(82)90158-1

data_9016544
_publ_section_title
;
 Synthese et caracterisation de nouvelles phases du diagramme (K ou Na)-Bi-O
 _cod_database_code 1004129
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              1235
_journal_page_last               1243
_journal_paper_doi               10.1016/0025-5408(82)90158-1
_journal_volume                  17
_journal_year                    1982
_chemical_formula_sum            'Bi K O3'
_space_group_IT_number           201
_symmetry_space_group_name_Hall  'P 2 2 3 -1n'
_symmetry_space_group_name_H-M   'P n -3 :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.035
_cell_length_b                   10.035
_cell_length_c                   10.035
_cell_formula_units_Z            12
_cell_volume                     1010.537
_database_code_amcsd             0014299
_exptl_crystal_density_diffrn    5.838
_cod_duplicate_entry             1004129
_cod_original_sg_symbol_H-M      'P n 3'
_cod_original_formula_sum        'K Bi O3'
_cod_database_code               9016544
_amcsd_formula_title             'Bi H0.5 K O3.25'
Crystal chemistry of chromian pumpellyite from Osayama, Okayama Prefecture, Japan Sample: ocp0604
Hamada, M.; Akasaka, M.; Seto, S.; Makino, K.; American Mineralogist 95 (2010) 1294–1304; doi:10.2138/am.2010.3376

data_9016545
_publ_section_title
;
 Crystal chemistry of chromian pumpellyite from Osayama, Okayama Prefecture, Japan
 Sample: ocp0604
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1294
_journal_page_last               1304
_journal_paper_doi               10.2138/am.2010.3376
_journal_volume                  95
_journal_year                    2010
_chemical_compound_source        'Osayama ultramafic body, Okayama, Japan'
_chemical_formula_sum
'Al2.22 Ca2 Cr0.27 Fe0.05 H2 Mg0.45 Mn0.01 O14 Si3'
_chemical_name_mineral           Pumpellyite-(Mg)
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 97.540
_cell_angle_gamma                90
_cell_length_a                   19.0935
_cell_length_b                   5.900
_cell_length_c                   8.810
_cell_formula_units_Z            4
_cell_volume                     983.880
_database_code_amcsd             0017598
_exptl_crystal_density_diffrn    3.231
_cod_original_formula_sum
'Ca2 Mg.45 Mn.01 Fe.05 Cr.27 Al2.22 Si3 O14 H2'
_cod_database_code               9016545
Structure cristalline de la manganite. _cod_database_code 1011020
Garrido, J.; Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences 200 (1935) 69–71; doi:

data_9016546
_publ_section_title
;
 Structure cristalline de la manganite.
 _cod_database_code 1011020
;
_journal_name_full
'Comptes Rendus Hebdomadaires des Seances de l'Academie des Sciences'
_journal_page_first              69
_journal_page_last               71
_journal_volume                  200
_journal_year                    1935
_chemical_formula_sum            'Mn O2'
_chemical_name_mineral           Manganite
_space_group_IT_number           58
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.42
_cell_length_b                   5.23
_cell_length_c                   2.87
_cell_formula_units_Z            2
_cell_volume                     66.345
_database_code_amcsd             0017927
_exptl_crystal_density_diffrn    4.352
_cod_duplicate_entry             1011020
_cod_original_formula_sum        'O2 Mn'
_cod_database_code               9016546
Microtwinning hypothesis for a more ordered vaterite model Note: Meyer (1959) model, not preferred
Le Bail, A.; Ouhenia, S.; Chateigner, D.; Powder Diffraction 26 (2011) 16–21; doi:10.1154/1.3552994

data_9016547
_publ_section_title
;
 Microtwinning hypothesis for a more ordered vaterite model
 Note: Meyer (1959) model, not preferred
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              16
_journal_page_last               21
_journal_paper_doi               10.1154/1.3552994
_journal_volume                  26
_journal_year                    2011
_chemical_compound_source        Synthetic
_chemical_formula_sum            'C Ca O3'
_chemical_name_mineral           Vaterite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   4.1291
_cell_length_b                   7.1581
_cell_length_c                   8.4764
_cell_formula_units_Z            4
_cell_volume                     250.533
_database_code_amcsd             0019140
_exptl_crystal_density_diffrn    2.654
_cod_original_formula_sum        'Ca C O3'
_cod_database_code               9016547
Structural and conductivity properties of Bi(0.775) Ln(0.225) O1.5 oxide conductors (Ln = La, Pr, Nd, Sm, Eu, Gd, Tb, Dy) with rhombohedral Bi-Sr-O type _cod_database_code 1004142
Drache, M.; Obbade, S.; Wignacourt, J.; Conflant, P.; Journal of Solid State Chemistry 142 (1999) 349–359; doi:10.1006/jssc.1998.8043

data_9016548
_publ_section_title
;
 Structural and conductivity properties of Bi(0.775) Ln(0.225) O1.5
 oxide conductors (Ln = La, Pr, Nd, Sm, Eu, Gd, Tb, Dy) with
 rhombohedral Bi-Sr-O type
 _cod_database_code 1004142
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              349
_journal_page_last               359
_journal_paper_doi               10.1006/jssc.1998.8043
_journal_volume                  142
_journal_year                    1999
_chemical_formula_sum            'Bi2.325 Dy0.675 O4.5'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   3.9649
_cell_length_b                   3.9649
_cell_length_c                   27.29599
_cell_formula_units_Z            3
_cell_volume                     371.616
_database_code_amcsd             0013966
_exptl_crystal_density_diffrn    8.949
_cod_duplicate_entry             1004142
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'Bi2.325 Dy.675 O4.5'
_cod_database_code               9016548
_amcsd_formula_title             'Bi0.775 Dy0.225 O1.5'
The structure of FeCl2 at high pressures Note: P = 6.40 kbar
Vettier, C.; Yelon, W. B.; Journal of Physics and Chemistry of Solids 36 (1975) 401–405; doi:10.1016/0022-3697(75)90065-7

data_9016549
_publ_section_title
;
 The structure of FeCl2 at high pressures
 Note: P = 6.40 kbar
;
_journal_name_full               'Journal of Physics and Chemistry of Solids'
_journal_page_first              401
_journal_page_last               405
_journal_paper_doi               10.1016/0022-3697(75)90065-7
_journal_volume                  36
_journal_year                    1975
_chemical_formula_sum            'Cl2 Fe'
_chemical_name_mineral           Lawrencite
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_length_a                   3.585
_cell_length_b                   3.585
_cell_length_c                   5.735
_cell_formula_units_Z            1
_cell_volume                     63.833
_database_code_amcsd             0018602
_exptl_crystal_density_diffrn    3.297
_cod_original_formula_sum        'Fe Cl2'
_cod_database_code               9016549
Structure refinement of Ag-free heyrovskyite from Vulcano (Aeolian Islands, Italy)
Pinto, D.; Balic-Zunic T; Garavelli, A.; Vurro, F.; American Mineralogist 96 (2011) 1120–1128; doi:10.2138/am.2011.3635

data_9016550
_publ_section_title
;
 Structure refinement of Ag-free heyrovskyite from Vulcano (Aeolian Islands, Italy)
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1120
_journal_page_last               1128
_journal_paper_doi               10.2138/am.2011.3635
_journal_volume                  96
_journal_year                    2011
_chemical_compound_source
'La Fossa crater, Vulcano (Aeolian Islands, Italy)'
_chemical_formula_sum            'Bi2.12 Pb5.828 S8.7 Se0.3'
_chemical_name_mineral           Heyrovskyite
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-B 2 2b'
_symmetry_space_group_name_H-M   'B b m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   13.7498
_cell_length_b                   31.5053
_cell_length_c                   4.1475
_cell_formula_units_Z            4
_cell_volume                     1796.662
_database_code_amcsd             0018391
_exptl_crystal_density_diffrn    7.221
_cod_original_formula_sum        'Pb5.828 Bi2.12 S8.7 Se.3'
_cod_database_code               9016550
High-pressure study of a natural cancrinite Note: P = 5.73 GPa
Lotti, P.; Gatta, G. D.; Rotiroti, N.; Camara, F.; American Mineralogist 97 (2012) 872–882; doi:10.2138/am.2012.4039

data_9016551
_publ_section_title
;
 High-pressure study of a natural cancrinite
 Note: P = 5.73 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              872
_journal_page_last               882
_journal_paper_doi               10.2138/am.2012.4039
_journal_volume                  97
_journal_year                    2012
_chemical_compound_source        Cameroun
_chemical_formula_sum            'C0.88 H2 Al3 Ca0.438 Na3.522 O15.64 Si3'
_chemical_name_mineral           Cancrinite
_space_group_IT_number           173
_symmetry_space_group_name_Hall  'P 6c'
_symmetry_space_group_name_H-M   'P 63'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   12.278
_cell_length_b                   12.278
_cell_length_c                   4.876
_cell_volume                     636.575
_database_code_amcsd             0019033
_exptl_crystal_density_diffrn    2.747
_cod_original_formula_sum        'Si3 O15.64 Al3 Na3.522 Ca.438 C.88 H2'
_cod_database_code               9016551